"Instructions on the deforming paint scheme applied in factory conditions
The camouflage is painted on using mixed paints of the following colours at the viscosity of interior paint.
- Green "gray-earth" colour #4K
- Dark "brown" colour #6K
- Khaki "yellow" colour #7K
- General army 4BO khaki green paint
- Prepare the item for painting using the typical method at the factory. If putty is used, it must have anti-corrosive properties no worse than red ochre primer.
- Apply red ochre primer with natural drying oils (or Oksol NKTP OST 7474/581)
The recommended concentrations of the primer (OST 7814/753) are as follows:
- 40% dry primer (or appropriate amount of mixed primer)
- 55% of natural drying oil
- 5% dessicant #64
The primer is applied using the commonly used method at the factory, depending on equipment. After primer is applied, the item should be dried. If possible, dry in hot conditions at 80 degrees for 2 hours.
- The first colour layer is applied with thick paints mixed with natural drying oil or Oksol drying oil in the following (approximate) ratios:
- 25 parts of oil by weight for 100 parts of colour #4K, produced experimentally at the Svobodniy Trud factory
- 40 parts of oil by weight for 100 parts of colour #6K, produced experimentally at the Svobodniy Trud factory
- 25 parts of oil by weight for 100 parts of colour #7K, produced experimentally at the Svobodniy Trud factory
- For 4BO paint, produced with different oil contents at different factories, use 30-50 parts of oil by weight for 100 parts of paint.
Note: this consistency is for painting with a brush. If using an airbrush, dilute to necessary viscosity with white spirits.
- The second colour layer is applied with thick paints mixed not with drying oil, but with white spirits or turpentine. While painting, continuously add the solvent to compensate for it evaporating, bringing the paint to initial viscosity.